Properties of Complex Inorganic Solids 2 pp 473-478 | Cite as

# Dynamical Lattice Instabilities in Alloy Phase Diagrams

Chapter

## Abstract

*Ab initio*electron structure calculations can accurately give total energies of solids in assumed atomic configurations for which there are no experimental data. As an example, one may calculate the total energy of silicon and germanium not only in the observed and stable diamond-type lattice structure but also in body centred cubic, face centred cubic, hexagonal close packed and other structures.1 Similarly the difference in cohesive energy between bcc, fcc and hcp lattice structures can be obtained across a transition-metal row in the Periodic Table.2 As another example, one may find the vacancy formation energy in 3d-, 4d- and 5d-transition metals when they are assumed to have a bcc structure and compare that with the results in an assumed fcc structure.3 In all such calculations, the atomic positions are kept fixed in a certain lattice structure, i.e. bcc, fcc, hcp etc. However many of these structures, for a given chemical composition, are dynamically unstable. The well-known conditions for elastic stability under shear, in a lattice of cubic symmetry, are4

$$
{{c}_{{44}}} > 0;\quad C' = ({{c}_{{11}}} - {{c}_{{12}}})/2 > 0
$$

(1)

*c*

_{ ij }are single-crystal elastic constants. Even if these inequalities referring to long-wavelength deformations are fulfilled, there may be instabilities under a lattice modulation of short wavelength. To ensure stability of a lattice for any small displacement of the atoms from their assumed equilibrium positions, all phonon frequencies

*ω*(

*,*

**q***s*) of wavevectors

*and mode indices*

**q***s*must be real, i.e.,

$$
{{\omega }^{2}}(q,s) > 0
$$

(2)

## Keywords

Alloy Phase Diagram Phonon Frequency Lattice Instability Vacancy Formation Energy Pressure Phase Diagram
These keywords were added by machine and not by the authors. This process is experimental and the keywords may be updated as the learning algorithm improves.

## Preview

Unable to display preview. Download preview PDF.

## References

- 1.M.T. Yin and M.L. Cohen,
*Theory of static structural properties, crystal stability, and phase transformations: Application to Si and Ge*, Phys. Rev. B 26:5668 (1982).ADSGoogle Scholar - 2.H. Skriver,
*Crystal structure from one-electron theory*, Phys. Rev. B 31:1909 (1985).ADSGoogle Scholar - 3.P.A. Korzhavyi, I.A. Abrikosov, B. Johansson, A.V. Ruban, and H.L. Skriver,
*First-principles calculations of the vacancy formation energy in transition and noble metals*, Phys. Rev. B 59:11693 (1999).ADSGoogle Scholar - 4.G. Grimvall,
*Thermophysical Properties of Materials*, North-Holland, Amsterdam (1999).Google Scholar - 5.J.M. Wills, O. Eriksson, P. Söderlind, and A.M. Boring,
*Trends of the elastic constants of cubic transition metals*, Phys. Rev. Lett. 68:2802 (1992).ADSCrossRefGoogle Scholar - 6.P.J. Craievich, M. Weinert, J.M. Sanchez, and R.E. Watson,
*Local stability of non-equilibrium phases*, Phys. Rev. Lett. 72:3076 (1994).ADSCrossRefGoogle Scholar - 7.P.J. Craievich, J.M. Sanchez, R.E. Watson, and M. Weinert,
*Structural instabilities of excited phases*, Phys. Rev. B 55:787 (1997).ADSGoogle Scholar - 8.G. Grimvall,
*Reconciling ab initio and semiempirical approaches to lattice stabilities*, Ber. Bunsenges. Phys.Chem. 102:1083 (1998).CrossRefGoogle Scholar - 9.T. Kraft, P.M. Marcus, M. Methfessel, and M. Scheffler,
*Elastic constants of Cu and the instability of its bcc structure*, Phys. Rev. B 48:5886 (1993).ADSGoogle Scholar - 10.P.J. Craievich and J.M. Sanchez,
*Vibrational free energy in the Ni-Cr system*, Comput. Mater. Sci. 8:92 (1997).CrossRefGoogle Scholar - 11.J.A. Moriarty and J.D. Althoff,
*First-principles temperature-pressure phase diagram of magnesium*Phys. Rev. B 51:5609 (1995).ADSGoogle Scholar - 12.K. Persson, M. Ekman, and G. Grimvall,
*Dynamical and thermodynamical instabilities in the disordered rhenium-tungsten system*, Phys. Rev. B60 (1999), in press.Google Scholar - 13.K. Einarsdotter, B. Sadigh, G. Grimvall, and V. Ozoliņš,
*Phonon instabilities in fcc and bcc tungsten*, Phys. Rev. Lett. 79:2073 (1997).ADSCrossRefGoogle Scholar - 14.V. Ozoliņš , and A. Zunger,
*Theory of systematic absence of NaCl-type (ß-Sn-type) high pressure phases in covalent (ionic) semiconductors*, Phys. Rev. Lett. 82:767 (1999).ADSCrossRefGoogle Scholar - 15.K.-M. Ho, C.L. Fu, and B.N. Harmon,
*Vibrational frequencies via total-energy calculations. Applications to transition metals*, Phys. Rev. B 29:1575 (1984).ADSGoogle Scholar - 16.A. Fernández Guillermet, V. Ozoliņš, G. Grimvall, and M. Körling,
*Phase stabilities in the Pt-W system: Thermodynamic and electronic-structure calculations*, Phys. Rev. B 51:10364 (1995).ADSGoogle Scholar - 17.M. Ekman, K. Persson, and G. Grimvall,
*Phase diagram and lattice instability in tungsten-rhenium alloys*, J. Nucl. Mater. (1999), in press.Google Scholar

## Copyright information

© Springer Science+Business Media New York 2000